Characterisation of the (Y1?xLax)2Ti2O7 system by powder diffraction and nuclear magnetic resonance methods
Harvey, Elizabeth J.; Ashbrook, Sharon E.; Lumpkin, Gregory R.; Redfern, Simon A. T.; Journal of Materials Chemistry 16 (2006) 4665–; doi:10.1039/b608053g

data_7203534
_publ_section_title
;
 Characterisation of the (Y1?xLax)2Ti2O7 system by powder diffraction
 and nuclear magnetic resonance methods
;
_journal_issue                   48
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              4665
_journal_paper_doi               10.1039/b608053g
_journal_volume                  16
_journal_year                    2006
_chemical_compound_source        Synthetic
_chemical_formula_structural     Y0.15La1.85
_chemical_formula_sum            'La1.85 O7 Ti2 Y0.15'
_chemical_formula_weight         478.11
_chemical_melting_point_gt       1300
_chemical_name_common            'Yttrium Lanthanum Titanate'
_chemical_name_systematic        'Yttrium Lanthanum Titanate'
_space_group_IT_number           4
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_audit_creation_date             2006-03-13T15:33
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2006-03-13T15:33 Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 98.649(19)
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   7.7889(4)
_cell_length_b                   5.53193(26)
_cell_length_c                   13.0091(9)
_cell_volume                     554.16(6)
_computing_structure_refinement  GSAS
_pd_block_id
2006-03-13T15:33|YLATI_0_925_2MK2|E_Harvey|d8XRD
_pd_phase_name
'from C:/gsas/GSASace/isis251104/Schmalle_La2Ti2O7(best)_72433.cif'
_refine_ls_goodness_of_fit_all   0.85
_refine_ls_matrix_type           full
_refine_ls_number_parameters     18
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          2.36
_refine_ls_shift/su_mean         0.38
_cod_data_source_file            b608053g.txt
_cod_data_source_block           YLATI_0_925_2MK2_publ
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/adriana/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (354
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/adriana/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (284 times).

Automatic conversion script
Id: cif_fix_enum 1555 2011-01-17 13:19:09Z saulius 

The following automatic conversions were performed:

'_chemical_melting_point' tag was changed to
'_chemical_melting_point_gt' since the value was specified 'more
than' ('>') a certain temperature. The value '>1300' was changed to
'1300' - it should be numeric and without a unit designator.

Automatic conversion script
Id: cif_fix_values 1569 2011-02-09 13:29:24Z adriana 
;
_cod_original_cell_volume        554.16(7)
_cod_original_sg_symbol_H-M      'P 21'
_cod_database_code               7203534